Presentation on theme: "BY Assistant Professor Dr. Akram R. Jabur Department of Materials Eng. University Of Technology."— Presentation transcript:
BY Assistant Professor Dr. Akram R. Jabur Department of Materials Eng. University Of Technology
Microstructure Evaluation Learning objectives 1.Learn sample preparation for microstructure evaluation 2.Learn about the microscopes used to view microstructures Microstructure evaluation Steps for sample preparation not complicated, but skill is required Not just a research tool Reveals a great deal of information about a metal and the mechanical and thermal processes to which it has been exposed Microstructure information useful for Supplier evaluation Process development Competitive analysis Root cause analysis
Resin Mount Sample Sample cut up if too large to fit inside container Containers 25 to 50 mm (1 to 2 inches) diameter 25 mm Container Sample
Polishing Wheels Grind and Polish 1.Sample surface ground 2.Sample polished to mirror finish Polishing media is paste or slurry Side view Top view Mounted sample
Sample Etchant Etch to reveal microstructure features Etchant chemical used depends on the metal
Optical Microscope Use light (optical) microscopes to observe microstructures Up to about 2000x magnification At 1000x 10 m appears as 10 mm
Cold rolled and annealed brass Micrographs Cold rolled Annealed 550 C (1004 F) Annealed 650 C (1202 F) in.
TEM constructed in 1931 Von Ardenne first STEM in 1938 by rastering the electron beam in a TEM Zworykin et al. 1942, first SEM for bulk samples 1965 first commercial SEM by Cambridge Scientific Instruments Resolution at that time ~ 50 nm : Today < 1 nm Morphology only at that time : Today analytical instrument
It is a microscope that produces an image by using an electron beam that scans the surface of a specimen inside a vacuum chamber. What can we study in a SEM? Topography and morphology Chemistry Crystallography Orientation of grains In-situ experiments: Reactions with atmosphere Effects of temperature “Easy” sample preparation!! “Big” samples!
Scanning Electron Microscope (SEM) Image features less than 1 m ( ”) Uses electrons to form an image 100x to 100,000x magnification Vacuum chamber
AFM Cantilever TipAnt HeadBlood Cells Diamond Thin Film (Numerous Multifaceted Micro- crystals) Microstructure of a plain carbon steel that contains 0.44 wt% of carbon Calcium Phosphate Crystal
The instrument in brief
electron gun (filament) electromagnetic optics scan coils sample stage detectors vacuum system computer hardware and software (not trivial!!)
We want many electrons per time unit per area (high current density) and as small electron spot as possible Traditional guns: thermionic electron gun (electrons are emitted when a solid is heated) W-wire, LaB 6 -crystal Modern: field emission guns (FEG) (cold guns, a strong electric field is used to extract electrons) Single crystal of W, etched to a thin tip
Secondary electron detector: (Everhart-Thornley) Backscattered electron detector: (Solid-State Detector) Our traditional detectors Secondary electrons: Everhart-Thornley Detector Backscattered electrons: Solid State Detector X-rays: Energy dispersive spectrometer (EDS)
The SEM uses electrons instead of light to form an image. A beam of electrons is produced at the top of the microscope by heating of a metallic filament. The electron beam follows a vertical path through the column of the microscope. It makes its way through electromagnetic lenses which focus and direct the beam down towards the sample. Once it hits the sample, other electrons ( backscattered or secondary ) are ejected from the sample. Detectors collect the secondary or backscattered electrons, and convert them to a signal that is sent to a viewing screen similar to the one in an ordinary television, producing an image.backscatteredsecondaryproducing an image.
156 electrons! Image Detector Electron gun 288 electrons!
The incident electron beam is scattered in the sample, both elastically and inelastically This gives rise to various signals that we can detect (more on that on next slide) Interaction volume increases with increasing acceleration voltage and decreases with increasing atomic number
Where does the signals come from? Diameter of the interaction volume is larger than the electron spot resolution is poorer than the size of the electron spot
Generated from the collision between the incoming electrons and the loosely bonded outer electrons Low energy electrons (~10-50 eV) Only SE generated close to surface escape (topographic information is obtained) Number of SE is greater than the number of incoming electrons We differentiate between SE1 and SE2
The secondary electrons that are generated by the incoming electron beam as they enter the surface High resolution signal with a resolution which is only limited by the electron beam diameter SE2 The secondary electrons that are generated by the backscattered electrons that have returned to the surface after several inelastic scattering events SE2 come from a surface area that is bigger than the spot from the incoming electrons resolution is poorer than for SE1 exclusively Sample surface Incoming electrons SE2
A fraction of the incident electrons is retarded by the electro-magnetic field of the nucleus and if the scattering angle is greater than 180° the electron can escape from the surface High energy electrons (elastic scattering) Fewer BSE than SE We differentiate between BSE1 and BSE2
SE produces higher resolution images than BSE By placing the secondary electron detector inside the lens, mainly SE1 are detected Resolution of 1 – 2 nm is possible
Photons not electrons Each element has a fingerprint X-ray signal Poorer spatial resolution than BSE and SE Relatively few X-ray signals are emitted and the detector is inefficient relatively long signal collecting times are needed
Microstructure ranging from crystal structure to Engine components (SiC) XRD,TEM,STM SEMOM Grain I Grain II atomic Valve Turbo charge 1
Best resolution that can be obtained: size of the electron spot on the sample surface The introduction of FEG has dramatically improved the resolution of SEM’s The volume from which the signal electrons are formed defines the resolution SE image has higher resolution than a BSE image Scanning speed: a weak signal requires slow speed to improve signal- to-noise ratio when doing a slow scan drift in the electron beam can affect the accuracy of the analysis
References Fundamentals of materials Science and Engineering – William D. Callister Physical Metallurgy – Robert W. Cahn Physical Metallurgy and Advanced Materials – R. E. Smallman Physical Metallurgy Principles – Robert E. Reedhill Thank You